```14-1
CHAPTER 14
POLYMER STRUCTURES
PROBLEM SOLUTIONS
Hydrocarbon Molecules
Polymer Molecules
The Chemistry of Polymer Molecules
14.1 The repeat unit structures called for are sketched below.
(a) Polychlorotrifluoroethylene
(b) Poly(vinyl alcohol)
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-21
14.19 (a) This portion of the problem asks us to determine the ratio of butadiene to acrylonitrile repeat
units in a copolymer having a weight-average molecular weight of 250,000 g/mol and a degree of polymerization of
4640. It first becomes necessary to calculate the average repeat unit molecular weight of the copolymer, m , using
Equation 14.6 as
m =
Mn
DP
250, 000 g/mol
= 53.88 g/mol
4640
=
If we designate fb as the chain fraction of butadiene repeat units, since the copolymer consists of only two repeat
unit types, the chain fraction of acrylontrile repeat units fa is just 1 – fb. Now, Equation 14.7 for this copolymer
may be written in the form
m = f b mb + f a ma = f b mb + (1 − f b )ma
in which mb and ma are the repeat unit molecular weights for butadiene and acrylontrile, respectively. These values
are calculated as follows:
mb = 4(AC) + 6(AH) = 4(12.01 g/mol) + 6(1.008 g/mol) = 54.09 g/mol
ma = 3(AC) + 3(AH) + (AN) = 3(12.01 g/mol) + 3(1.008 g/mol) + (14.01 g/mol)
= 53.06 g/mol.
Solving for fb in the above expression yields
fb =
m − ma
mb − ma
=
53.88 g/mol − 53.06 g/mol
= 0.80
54.09 g/mol − 53.06 g/mol
Furthermore, fa = 1 – fb = 1 – 0.80 = 0.20; or the ratio is just
fb
fa
=
0.80
= 4.0
0.20
(b) Of the possible copolymers, the only one for which there is a restriction on the ratio of repeat unit
types is alternating; the ratio must be 1:1. Therefore, on the basis of the result in part (a), the possibilities for this
copolymer are random, graft, and block.
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-20
14.18 For an alternating copolymer that has a number-average molecular weight of 100,000 g/mol and a
degree of polymerization of 2210, we are to determine one of the repeat unit types if the other type is ethylene. It is
first necessary to calculate m using Equation 14.6 as
m =
Mn
DP
=
100,000 g/mol
= 42.25 g/mol
2210
Since this is an alternating copolymer we know that chain fraction of each repeat unit type is 0.5; that is fe = fx =
0.5, fe and fx being, respectively, the chain fractions of the ethylene and unknown repeat units. Also, the repeat unit
molecular weight for ethylene is
ms = 2(AC) + 4(AH)
= 2(12.01 g/mol) + 4(1.008 g/mol) = 28.05 g/mol
Now, using Equation 14.7, it is possible to calculate the repeat unit weight of the unknown repeat unit type, mx.
Thus
mx =
=
m − f e me
fx
45.25 g/mol - (0.5)(28.05 g/mol)
= 62.45 g/mol
0.5
Finally, it is necessary to calculate the repeat unit molecular weights for each of the possible other repeat
unit types. These are calculated below:
mstyrene = 8(AC) + 8(AH) = 8(12.01 g/mol) + 8(1.008 g/mol) = 104.16 g/mol
mpropylene = 3(AC) + 6(AH) = 3(12.01 g/mol) + 6(1.008 g/mol) = 42.08 g/mol
mTFE = 2(AC) + 4(AF) = 2(12.01 g/mol) + 4(19.00 g/mol) = 100.02 g/mol
mVC = 2(AC) + 3(AH) + (ACl) = 2(12.01 g/mol) + 3(1.008 g/mol) + 35.45 g/mol = 62.49 g/mol
Therefore, vinyl chloride is the other repeat unit type since its m value is almost the same as the calculated mx.
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-19
14.17
This problem asks for us to calculate the number-average molecular weight of a random
poly(isobutylene-isoprene) copolymer. For the isobutylene repeat unit there are four carbon and eight hydrogen
atoms. Thus, its repeat unit molecular weight is
mIb = 4(AC) + 8(AH)
= (4)(12.01 g/mol) + (8)(1.008 g/mol) = 56.10 g/mol
The isoprene repeat unit is composed of five carbon and eight hydrogen atoms. Thus, its repeat unit molecular
weight is
mIp = 5(AC) + 8(AH)
= (5)(12.01 g/mol) + (8)(1.008 g/mol) = 68.11 g/mol
From Equation 14.7, the average repeat unit molecular weight is just
m = f Ib mIb + f Ip mIp
= (0.25)(56.10 g/mol) + (0.75)(68.11 g/mol) = 65.11 g/mol
Since DP = 1500 (as stated in the problem), M n may be computed using Equation 14.6 as
M n = m (DP) = (65.11 g/mol)(1500) = 97, 700 g/mol
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-18
14.16 For a poly(acrylonitrile-butadiene) alternating copolymer with a number-average molecular weight
of 1,000,000 g/mol, we are asked to determine the average number of acrylonitrile and butadiene repeat units per
molecule.
Since it is an alternating copolymer, the number of both types of repeat units will be the same. Therefore,
consider them as a single repeat unit, and determine the number-average degree of polymerization. For the
acrylonitrile repeat unit, there are three carbon atoms, three hydrogen atoms, and one nitrogen atom, while the
butadiene repeat consists of four carbon atoms and six hydrogen atoms. Therefore, the acrylonitrile-butadiene
combined repeat unit weight is just
m = 7(AC) + 9(AH) + 1(AN)
= (7)(12.01 g/mol) + (9)(1.008 g/mol) + (14.01 g/mol) = 107.15 g/mol
From Equation 14.6, the degree of polymerization is just
DP =
Mn
m
=
1,000, 000 g/mol
= 9333
107.15 g/mol
Thus, there is an average of 9333 of both repeat unit types per molecule.
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-17
Copolymers
14.15 This problem asks for sketches of the repeat unit structures for several alternating copolymers.
(a) For poly(ethylene-propylene)
(c) For poly(isobutylene-isoprene)
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-16
14.14 (a) It is not possible to grind up and reuse phenol-formaldehyde because it is a network thermoset
polymer and, therefore, is not amenable to remolding.
(b) Yes, it is possible to grind up and reuse polypropylene since it is a thermoplastic polymer, will soften
when reheated, and, thus, may be remolded.
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-15
Thermoplastic and Thermosetting Polymers
14.13 This question asks for comparisons of thermoplastic and thermosetting polymers.
(a) Thermoplastic polymers soften when heated and harden when cooled, whereas thermosetting polymers,
harden upon heating, while further heating will not lead to softening.
(b) Thermoplastic polymers have linear and branched structures, while for thermosetting polymers, the
structures will normally be network or crosslinked.
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-14
14.12 This problem asks for us to sketch cis and trans structures for butadiene and chloroprene.
(a) The structure for cis polybutadiene (Table 14.5) is
The structure of trans butadiene is
(b) The structure of cis chloroprene (Table 14.5) is
The structure of trans chloroprene is
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-13
Molecular Configurations
14.11 We are asked to sketch portions of a linear polypropylene molecule for different configurations
(using two-dimensional schematic sketches).
(a) Syndiotactic polypropylene
(b) Atactic polypropylene
(c) Isotactic polypropylene
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-10
14.8 (a) For chlorinated polyethylene, we are asked to determine the weight percent of chlorine added for
8% Cl substitution of all original hydrogen atoms. Consider 50 carbon atoms; there are 100 possible side-bonding
sites. Ninety-two are occupied by hydrogen and eight are occupied by Cl. Thus, the mass of these 50 carbon atoms,
mC, is just
mC = 50(AC) = (50)(12.01 g/mol) = 600.5 g
Likewise, for hydrogen and chlorine,
mH = 92(AH) = (92)(1.008 g/mol) = 92.74 g
mCl = 8(ACl) = (8)(35.45 g/mol) = 283.60 g
Thus, the concentration of chlorine, CCl, is determined using a modified form of Equation 4.3 as
CCl =
=
mCl
mC + mH + mCl
x 100
283.60 g
x 100 = 29.0 wt%
600.5 g + 92.74 g + 283.60 g
(b) Chlorinated polyethylene differs from poly(vinyl chloride), in that, for PVC, (1) 25% of the sidebonding sites are substituted with Cl, and (2) the substitution is probably much less random.
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-9
14.7 This problem asks if it is possible to have a poly(vinyl chloride) homopolymer with the given
molecular weight data and a degree of polymerization of 1120. The appropriate data are given below along with a
computation of the number-average molecular weight.
Molecular wt.
Range
Mean Mi
xi
8,000-20,000
14,000
0.05
700
20,000-32,000
26,000
0.15
3900
32,000-44,000
38,000
0.21
7980
44,000-56,000
50,000
0.28
14,000
56,000-68,000
62,000
0.18
11,160
68,000-80,000
74,000
0.10
7440
80,000-92,000
86,000
0.03
xiMi
2580
_________________________
Mw =
∑ xi M i
= 47, 720 g/mol
For PVC, from Table 14.3, each repeat unit has two carbons, three hydrogens, and one chlorine. Thus,
m = 2(AC) + 3(AH) + (ACl)
= (2)(12.01 g/mol) + (3)(1.008 g/mol) + (35.45 g/mol) = 62.49 g/mol
Now, we will compute the degree of polymerization using Equation 14.6 as
DP =
Mn
m
=
47,720 g/mol
= 764
62.49 g/mol
Thus, such a homopolymer is not possible since the calculated degree of polymerization is 764 not 1120.
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-8
The repeat unit molecular weights of the polymers listed in Table 14.3 are as follows:
Polyethylene--28.05 g/mol
Poly(vinyl chloride)--62.49 g/mol
Polytetrafluoroethylene--100.02 g/mol
Polypropylene--42.08 g/mol
Polystyrene--104.14 g/mol
Poly(methyl methacrylate)--100.11 g/mol
Phenol-formaldehyde--133.16 g/mol
Nylon 6,6--226.32 g/mol
PET--192.16 g/mol
Polycarbonate--254.27 g/mol
Therefore, polytetrafluoroethylene is the material since its repeat unit molecular weight is closest to that calculated
above.
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-7
14.6 (a) From the tabulated data, we are asked to compute M n , the number-average molecular weight.
This is carried out below.
Molecular wt.
Range
Mean Mi
xi
xiMi
8,000-20,000
14,000
0.05
700
20,000-32,000
26,000
0.15
3900
32,000-44,000
38,000
0.21
7980
44,000-56,000
50,000
0.28
14,000
56,000-68,000
62,000
0.18
11,160
68,000-80,000
74,000
0.10
7400
80,000-92,000
86,000
0.03
2580
_________________________
Mn =
∑ xi M i
= 47,720 g/mol
(b) From the tabulated data, we are asked to compute M w , the weight-average molecular weight. This
determination is performed as follows:
Molecular wt.
Range
Mean Mi
wi
wiMi
8,000-20,000
14,000
0.02
280
20,000-32,000
26,000
0.08
2080
32,000-44,000
38,000
0.17
6460
44,000-56,000
50,000
0.29
14,500
56,000-68,000
62,000
0.23
14,260
68,000-80,000
74,000
0.16
11,840
80,000-92,000
86,000
0.05
4300
_________________________
Mw =
∑ wi M i
= 53,720 g/mol
(c) We are now asked if the degree of polymerization is 477, which of the polymers in Table 14.3 is this
material? It is necessary to compute m in Equation 14.6 as
m =
Mn
DP
=
47,720 g/mol
= 100.04 g/mol
477
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-6
m = 2(AC) + 4(AF)
= (2)(12.01 g/mol) + (4)(19.00 g/mol) = 100.02 g/mol
And
DP =
Mn
m
=
49,800 g/mol
= 498
100.02 g/mol
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-5
14.5 (a) From the tabulated data, we are asked to compute M n , the number-average molecular weight.
This is carried out below.
Molecular wt
Range
Mean Mi
xi
xiMi
10,000-20,000
15,000
0.03
450
20,000-30,000
25,000
0.09
2250
30,000-40,000
35,000
0.15
5250
40,000-50,000
45,000
0.25
11,250
50,000-60,000
55,000
0.22
12,100
60,000-70,000
65,000
0.14
9100
70,000-80,000
75,000
0.08
6000
80,000-90,000
85,000
0.04
3400
____________________________
M n = ∑ xi M i = 49,800 g/mol
(b) From the tabulated data, we are asked to compute M w , the weight-average molecular weight.
Molecular wt.
Range
Mean Mi
wi
wiMi
10,000-20,000
15,000
0.01
150
20,000-30,000
25,000
0.04
1000
30,000-40,000
35,000
0.11
3850
40,000-50,000
45,000
0.23
10,350
50,000-60,000
55,000
0.24
13,200
60,000-70,000
65,000
0.18
11,700
70,000-80,000
75,000
0.12
9000
80,000-90,000
85,000
0.07
5950
___________________________
Mw =
wi M i = 55,200 g/mol
∑
(c) Now we are asked to compute the degree of polymerization, which is possible using Equation 14.6.
For polytetrafluoroethylene, the repeat unit molecular weight is just
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-4
14.4 (a) The repeat unit molecular weight of polypropylene is called for in this portion of the problem.
For polypropylene, from Table 14.3, each repeat unit has three carbons and six hydrogens. Thus,
m = 3(AC) + 6(AH)
= (3)(12.01 g/mol) + (6)(1.008 g/mol) = 42.08 g/mol
(b)
We are now asked to compute the number-average molecular weight. Since the degree of
polymerization is 15,000, using Equation 14.6
M n = (DP)m = (15, 000)(42.08 g/mol) = 631, 000 g/mol
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-3
14.3 We are asked to compute the degree of polymerization for polystyrene, given that the numberaverage molecular weight is 500,000 g/mol. The repeat unit molecular weight of polystyrene is just
m = 8(AC) + 8(AH)
= (8)(12.01 g/mol) + (8)(1.008 g/mol) = 104.14 g/mol
Now it is possible to compute the degree of polymerization using Equation 14.6 as
DP =
Mn
m
=
500, 000 g/mol
= 4800
104.14 g/mol
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-2
Molecular Weight
14.2 Repeat unit weights for several polymers are asked for in this problem.
(a) For polytetrafluoroethylene, each repeat unit consists of two carbons and four fluorines (Table 14.3).
If AC and AF represent the atomic weights of carbon and fluorine, respectively, then
m = 2(AC) + 4(AF)
= (2)(12.01 g/mol) + (4)(19.00 g/mol) = 100.02 g/mol
(b) For poly(methyl methacrylate), from Table 14.3, each repeat unit has five carbons, eight hydrogens,
and two oxygens. Thus,
m = 5(AC) + 8(AH) + 2(AO)
= (5)(12.01 g/mol) + (8)(1.008 g/mol) + (2)(16.00 g/mol) = 100.11 g/mol
(c) For nylon 6,6, from Table 14.3, each repeat unit has twelve carbons, twenty-two hydrogens, two
nitrogens, and two oxygens. Thus,
m = 12(AC) + 22(AH) + 2(AN) + 2(AO)
= (12)(12.01 g/mol) + (22)(1.008 g/mol) + (2)(14.01 g/mol) + (2)(16.00 g/mol)
= 226.32 g/mol
(d) For poly(ethylene terephthalate), from Table 14.3, each repeat unit has ten carbons, eight hydrogens,
and four oxygens. Thus,
m = 10(AC) + 8(AH) + 4(AO)
= (10)(12.01 g/mol) + (8)(1.008 g/mol) + (4)(16.00 g/mol) = 192.16 g/mol
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-33
14.29 This problem asks that we compute the diffusion flux at 350 K for water in polystyrene. It is first
necessary to compute the value of the permeability coefficient at 350 K. The temperature dependence of PM is
given in the problem statement, as follows:
⎛ Q ⎞
p
⎟
PM = PM exp ⎜⎜−
⎟
0
⎝ RT ⎠
And, incorporating values provided for the constants PM and Qp, we get
0
⎡
⎡
⎤
42,300 J/mol
(cm 3 STP)(cm) ⎤
⎥ exp ⎢−
PM = ⎢9.0 x 10-5
⎥
2
⎢⎣
⎣ (8.314 J/mol - K)(350 K) ⎦
cm - s - Pa ⎥⎦
= 4.4 x 10−11
(cm3 STP)(cm)
cm 2 - s - Pa
And, using Equation 14.9, the diffusion flux is equal to
J = PM
= 4.4 x 10-11
P −P
∆P
= PM 2 1
∆x
∆x
(cm3 STP)(cm) ⎛ 20,000 Pa - 1,000 Pa ⎞
⎟
⎜
⎠
3.0 cm
cm2 - s - Pa ⎝
= 2.8 x 10-7
(cm3 STP)
cm2 - s
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-32
14.28 This problem asks us to compute the permeability coefficient for carbon dioxide through high
density polyethylene at 325 K given a steady-state permeability situation. It is necessary for us to Equation 14.9 in
order to solve this problem. Rearranging this expression and solving for the permeability coefficient gives
PM =
J ∆x
J ∆x
=
∆P P2 − P1
Taking P1 = 2500 kPa (2,500,000 Pa) and P1 = 4000 kPa (4,000,000 Pa), the permeability coefficient of CO2
through HDPE is equal to
⎡
(cm 3 STP) ⎤
⎢2.2 x 10-8
⎥(5 cm)
⎢⎣
cm2 - s ⎥⎦
PM =
(4,000,000 Pa - 2,500, 000 Pa)
= 0.73 x 10-13
(cm3 STP)(cm)
cm2 - s - Pa
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-31
Diffusion in Polymeric Materials
14.27 This is a permeability problem in which we are asked to compute the diffusion flux of oxygen
through a 15-mm thick sheet of low density polyethylene. In order to solve this problem it is necessary to employ
Equation 14.9. The permeability coefficient of O2 through LDPE is given in Table 14.6 as 2.2 x 10-13 (cm3 STP)cm/cm2-s-Pa. Thus, from Equation 14.9
J = PM
P −P
∆P
= PM 2 1
∆x
∆x
and taking P1 = 150 kPa (150,000 Pa) and P2 = 2000 kPa (2,000,000 Pa) we get
⎡
(cm3 STP)(cm) ⎤ ⎛ 2,000,000 Pa - 150, 000 Pa ⎞
⎥⎜
= ⎢2.2 x 10-13
⎟
⎠
1.5 cm
⎢⎣
cm2 - s - Pa ⎥⎦ ⎝
= 2.7 x 10-6
(cm3 STP)
cm2 - s
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-30
ρs =
=
− ρc ρa
C (ρc − ρa ) − ρc
− (0.946 g /cm3)( 0.841 g /cm3 )
(0.746) (0.946 g /cm3 − 0.841 g /cm3) − 0.946 g /cm3
= 0.917 g/cm3
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-29
14.26
(a)
We are asked to compute the densities of totally crystalline and totally amorphous
% crystallinity
polypropylene (ρc and ρa from Equation 14.8). From Equation 14.8 let C =
, such that
100
C =
ρc (ρ s − ρa )
ρ s (ρc − ρa )
Rearrangement of this expression leads to
ρc (C ρ s − ρ s ) + ρcρa − C ρ sρa = 0
in which ρc and ρa are the variables for which solutions are to be found. Since two values of ρs and C are specified
in the problem, two equations may be constructed as follows:
ρc (C1 ρ s1 − ρ s1) + ρcρa − C1ρ s1ρa = 0
ρc (C 2 ρ s2 − ρ s 2 ) + ρcρa − C 2ρ s 2ρa = 0
In which ρs1 = 0.904 g/cm3, ρs2 = 0.895 g/cm3, C1 = 0.628, and C2 = 0.544. Solving the above two equations for
ρa =
=
(0.904
ρ s1 ρ s2 (C1 − C 2 )
C1 ρ s1 − C 2 ρ s 2
g /cm3)( 0.895 g /cm3) (0.628 − 0.544)
(0.628) (0.904 g /cm3) − (0.544) (0.895 g /cm3 )
= 0.841 g/cm3
And
ρc =
=
(0.904
ρ s1 ρ s2 (C 2 − C1 )
ρ s2 (C 2 − 1) − ρ s1(C1 − 1)
g /cm3)( 0.895 g /cm3) (0.544 − 0.628)
(0.895 g /cm3) (0.544 − 1.0) − (0.904 g /cm3) (0.628 − 1.0)
= 0.946 g/cm3
(b) Now we are asked to determine the density of a specimen having 74.6% crystallinity. Solving for ρs
from Equation 14.8 and substitution for ρa and ρc which were computed in part (a) yields
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-28
% crystallinity =
=
ρc (ρ s − ρa )
ρ s (ρc − ρa )
(1.450 g/cm3)(1.382 g/cm3
(1.382 g/cm3)(1.450 g/cm3
&times; 100
− 1.300 g/cm3 )
− 1.300 g/cm3)
&times; 100
= 57.4%
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-27
14.25 (a) We are asked to compute the densities of totally crystalline and totally amorphous poly(ethylene
% crystallinity
terephthalate) (ρc and ρa from Equation 14.8). From Equation 14.8 let C =
, such that
100
C =
ρc (ρ s − ρa )
ρ s (ρc − ρa )
Rearrangement of this expression leads to
ρc (C ρ s − ρ s ) + ρcρa − Cρ s ρa = 0
in which ρc and ρa are the variables for which solutions are to be found. Since two values of ρs and C are specified
in the problem statement, two equations may be constructed as follows:
ρc (C1 ρ s1 − ρ s1 ) + ρcρa − C1 ρ s1 ρa = 0
ρc (C2 ρ s2 − ρ s2 ) + ρcρa − C 2 ρ s2 ρa = 0
In which ρs1 = 1.408 g/cm3, ρs2 = 1.343 g/cm3, C1 = 0.743, and C2 = 0.312. Solving the above two equations for
ρa =
=
ρ s1 ρ s2 (C1 − C 2 )
C1 ρ s1 − C 2 ρ s2
(1.408 g/cm3)( 1.343 g/cm3)(0.743 − 0.312)
= 1.300 g/cm3
(0.743) (1.408 g/cm3 ) − (0.312) (1.343 g/cm3)
And
ρc =
=
ρ s1 ρ s2 (C 2 − C1)
ρ s2 (C 2 − 1) − ρ s1 (C1 − 1)
(1.408 g/cm3)( 1.343 g/cm3)(0.312 − 0.743)
= 1.450 g/cm3
3
3
(1.343 g/cm )(0.312 − 1.0) − (1.408 g/cm )(0.743 − 1.0)
(b) Now we are to determine the % crystallinity for ρs = 1.382 g/cm3. Again, using Equation 14.8
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-26
14.24 For this problem we are given the density of nylon 6,6 (1.213 g/cm3), an expression for the volume
of its unit cell, and the lattice parameters, and are asked to determine the number of repeat units per unit cell. This
computation necessitates the use of Equation 3.5, in which we solve for n. Before this can be carried out we must
first calculate VC, the unit cell volume, and A the repeat unit molecular weight. For VC
VC = abc 1 − cos 2 α − cos 2 β − cos 2 γ + 2 cos α cos β cos γ
= (0.497)(0.547)(1.729) 1 − 0.441 − 0.054 − 0.213 + 2 (0.664)(0.232)(0.462)
= 0.3098 nm3 = 3.098 x 10-22 cm3
The repeat unit for nylon 6,6 is shown in Table 14.3, from which the value of A may be determined as follows:
A = 12(AC) + 22(AH) + 2(AO) + 2(AN)
= 12(12.01 g/mol) + 22(1.008 g/mol) + 2(16.00 g/mol) + 2(14.01 g/mol)
= 226.32 g/mol
Finally, solving for n from Equation 3.5 leads to
n =
=
ρVC N A
A
(1.213 g/cm3 )( 3.098 x 10 -22 cm3/unit cell)( 6.023 x 10 23 repeat units/mol)
226.32 g/mol
= 1 repeat unit/unit cell
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-25
14.23 For each of four pairs of polymers, we are asked to (1) state whether it is possible to decide which is
more likely to crystallize; (2) if so, which is more likely and why; and (3) it is not possible to decide then why.
(a) No, it is not possible to decide for these two polymers. On the basis of tacticity, the isotactic PP is more
likely to crystallize than the atactic PVC. On the other hand, with regard to side-group bulkiness, the PVC is more
likely to crystallize.
(b) Yes, it is possible to decide for these two copolymers. The linear and syndiotactic polypropylene is
more likely to crystallize than crosslinked cis-isoprene since linear polymers are more likely to crystallize than
(c) Yes, it is possible to decide for these two polymers. The linear and isotactic polystyrene is more likely
to crystallize than network phenol-formaldehyde; network polymers rarely crystallize, whereas isotactic ones
crystallize relatively easily.
(d)
Yes, it is possible to decide for these two copolymers.
The block poly(acrylonitrile-isoprene)
copolymer is more likely to crystallize than the graft poly(chloroprene-isobutylene) copolymer. Block copolymers
crystallize more easily than graft ones.
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-24
Polymer Crystallinity
14.22 The tendency of a polymer to crystallize decreases with increasing molecular weight because as the
chains become longer it is more difficult for all regions along adjacent chains to align so as to produce the ordered
atomic array.
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-23
14.21 For a random poly(styrene-butadiene) copolymer in which M n = 350,000 g/mol and DP = 5000, we
are asked to compute the fractions of styrene and butadiene repeat units.
From Table 14.5, the styrene repeat unit has eight carbon and eight hydrogen atoms. Thus,
mst = (8)(12.01 g/mol) + (8)(1.008 g/mol) = 104.14 g/mol
Also, from Table 14.5, the butadiene repeat unit has four carbon and six hydrogen atoms, and
mbu = (4)(12.01 g/mol) + (6)(1.008 g/mol) = 54.09 g/mol
From Equation 14.7
m = f st mst + f bu mbu
Now, let x = fst, such that
m = 104.14x + (54.09)(1 − x)
since fst + fbu = 1. Also, from Equation 14.6
DP =
Mn
m
Or
5000 =
350,000 g / mol
[104.14 x + 54.09(1 − x)] g / mol
Solving for x leads to x = fst = f(styrene) = 0.32. Also,
f(butadiene) = 1 – x = 1 – 0.32 = 0.68
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
14-22
14.20 For a copolymer consisting of 35 wt% ethylene and 65 wt% propylene, we are asked to determine
the fraction of both repeat unit types.
In 100 g of this material, there are 35 g of ethylene and 65 g of propylene. The ethylene (C2H4) molecular
weight is
m(ethylene) = 2(AC) + 4(AH)
= (2)(12.01 g/mol) + (4)(1.008 g/mol) = 28.05 g/mol
The propylene (C3H6) molecular weight is
m(propylene) = 3(AC) + 6(AH)
= (3)(12.01 g/mol) + (6)(1.008 g/mol) = 42.08 g/mol
Therefore, in 100 g of this material, there are
35 g
= 1.25 mol of ethylene
28.05 g / mol
and
65 g
= 1.54 mol of propylene
42.08 g / mol
Thus, the fraction of the ethylene repeat unit, f(ethylene), is just
f (ethylene) =
1.25 mol
= 0.45
1.25 mol + 1.54 mol
Likewise,
f (propylene) =
1.54 mol
= 0.55
1.25 mol + 1.54 mol
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
```